Intercalation of Copper Phthalocyanine Within Bulk Graphite as a New Strategy Toward the Synthesis of CuO-Based CO Oxidation Catalysts Gaëlle Couvret, Ghislain Genay, Cerise Robert, Loic Michel, Valérie Caps
To cite this version:
Gaëlle Couvret, Ghislain Genay, Cerise Robert, Loic Michel, Valérie Caps. Intercalation of Copper Phthalocyanine Within Bulk Graphite as a New Strategy Toward the Synthesis of CuO-Based CO Oxidation Catalysts. Frontiers in Chemistry, Frontiers Media, 2020, 8, 10.3389/fchem.2020.00735. hal-02928127
HAL Id: hal-02928127 https://hal.archives-ouvertes.fr/hal-02928127 Submitted on 2 Sep 2020
HAL is a multi-disciplinary open access L’archive ouverte pluridisciplinaire HAL, est archive for the deposit and dissemination of sci- destinée au dépôt et à la diffusion de documents entific research documents, whether they are pub- scientifiques de niveau recherche, publiés ou non, lished or not. The documents may come from émanant des établissements d’enseignement et de teaching and research institutions in France or recherche français ou étrangers, des laboratoires abroad, or from public or private research centers. publics ou privés. ORIGINAL RESEARCH published: 31 August 2020 doi: 10.3389/fchem.2020.00735
Intercalation of Copper Phthalocyanine Within Bulk Graphite as a New Strategy Toward the Synthesis of CuO-Based CO Oxidation Catalysts
Gaëlle Couvret, Ghislain Genay, Cerise Robert, Loïc Michel and Valérie Caps*
ICPEES (Institut de Chimie et Procédés pour l’Energie, l’Environnement et la Santé), Université de Strasbourg - ECPM / CNRS UMR 7515, Strasbourg, France
Graphite is a widely available natural form of carbon with peculiar chemical and surface properties. It is essentially hydrophobic and consists in very stable stacks of graphene layers held together by highly delocalized π-π interactions. Its use in chemistry and in particular for catalytic applications requires modiﬁcation of its structure to increase its surface area. This is commonly achieved by harsh oxidation methods which also Edited by: modiﬁes the chemical composition of graphite and enables subsequent deposition of Svetlana Ivanova, University of Seville, Spain catalytic phases via common impregnation/reduction methods. Here we show that Reviewed by: copper phthalocyanine (CuPc) can be incorporated into unmodiﬁed bulk graphite by Vincent Blay, the straight-forward sonication of a dimethylformamide solution containing CuPc and The Ohio State University, graphite ﬂakes. Immobilization of the CuPc complex in the graphitic matrix is shown United States Jose Luis Santos Muñoz, to rely on π-π interactions between the Pc ligand and graphenic surfaces. This strong KU Leuven, Belgium CuPc-graphene interaction facilitates oxidation of the graphitic matrix upon oxidation of *Correspondence: the immobilized complex, as shown by thermogravimetric analysis in air. Nevertheless, Valérie Caps [email protected] a soft oxidation treatment can be designed to produce CuO nanoparticles (NPs) without degrading the dispersing graphitic matrix. These well-dispersed CuO NPs are shown Specialty section: (1) to decrease the degree of stacking of graphite in the solid-state by intercalation This article was submitted to Physical Chemistry and Chemical in-between graphitic stacks, (2) to be more easily reducible than bulk CuO, and (3) to Physics, be catalytically active for the oxidation of carbon monoxide. The higher mass-speciﬁc a section of the journal CO oxidation rates observed, as compared with CuO/alumina benchmarks, highlight the Frontiers in Chemistry beneﬁcial role of the carbon support and the relevance of this new strategy toward the Received: 11 May 2020 Accepted: 16 July 2020 design of copper oxide catalysts from copper phthalocyanine metal complexes. Published: 31 August 2020 Keywords: copper complexes, immobilization, controlled oxidation, catalytic CO oxidation, non-covalent Citation: interactions, exfoliation, graphite, graphene Couvret G, Genay G, Robert C, Michel L and Caps V (2020) Intercalation of Copper INTRODUCTION Phthalocyanine Within Bulk Graphite as a New Strategy Toward the Synthesis of CuO-Based CO Graphite is a naturally occurring, stable form of carbon. It is a highly crystalline, bulk, purely Oxidation Catalysts. carbonaceous material which combines high conductivity, high thermal stability, exceptional Front. Chem. 8:735. mechanical resistance, resistance to corrosion, and lightness. It is thus widely used in its bulk doi: 10.3389/fchem.2020.00735 form as electrodes and as component for refractories and for super-light materials. The world
Frontiers in Chemistry | www.frontiersin.org 1 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine resource is estimated to be around 800 million tons (U.S. Due to their redox chemistry, copper oxides are known to Geological Survey, Mineral commodity summaries 2020, p. 73), catalyze useful reactions such as the oxidation of CO (Wan which by far exceeds resources in metals and other elements. et al., 2008; Gawande et al., 2016). This reaction is of both On the nanoscale, it consists of stacks of graphene layers which practical importance (Waikar et al., 2019) and academic interest are held together by strong π interactions due to electron (Caps et al., 2008; Freund et al., 2011). It is indeed used for air delocalization over their extended aromatic networks (Wang depollution, as CO is toxic to human health (Soliman, 2019), and et al., 2015). It exhibits virtually no surface area and its use as for puriﬁcation of hydrogen fuel cells gas feed (Ivanova et al., a catalyst support thus generally requires exfoliation and surface 2010; Laveille et al., 2016). It is also a quite simple redox reaction functionalization (Cai et al., 2012). Exfoliation allows to break the that is catalyzed by metal oxides following a Mars van Krevelen stacks down to thinner stacks, ultimately to single layer graphene mechanism (Mars and van Krevelen, 1954). It can thus also be if needed, hence increasing the available surface which can be used to probe the reducibility of oxide catalysts (Laveille et al., used for subsequent deposition of metal nanostructures. Surface 2013). functionalization aims at providing reactive sites for decoration Here we show that an eﬃcient CuO/graphite CO oxidation with such active phases. catalyst can be prepared by soft oxidation of a strongly The most widely used exfoliation/functionalization method interacting CuPc/graphite precursor, with no need for extensive consists in harsh oxidation of the graphitic structure by strong exfoliation of graphite. First, we investigate the potentials of acids, sodium nitrate, and potassium permanganate following metal complexes, namely copper phthalocyanine and copper Hummers-type procedures (Hummers and Oﬀeman, 1958). In tetraphenylporphine (CuTPP), as precursors for the direct this approach, deep exfoliation of the structure results from a decoration of unmodiﬁed hydrophobic bulk graphite with drastic change in the chemical composition of the planes, namely functional copper phases, by screening various sonication- the introduction of out-of-plane, covalently-bound oxygen atoms based, organic exfoliation conditions in the liquid phase. Then, (Dreyer et al., 2014). The increased interlayer spacing is retained by combining thermogravimetric analysis (TGA) and Fourier- in the dry state. The resulting graphite oxide is water-soluble Transform Infra-Red (FTIR) studies, we show that copper and can further react with metal salts in solution. Metal ions phthalocyanine strongly interacts with the graphitic surface can thus easily be anchored onto the structure via surface and that it can be thermally oxidized to an easily reducible, oxygen groups. Graphene-supported metal nanoparticles are catalytically active cupric oxide phase, which is active for CO subsequently obtained in a third step by co-reduction of the oxidation both in the absence and in the presence of hydrogen. graphitic oxide matrix and the interacting metal ion (Goncalves et al., 2009). MATERIALS AND METHODS Organic dyes are also known to exfoliate and functionalize graphite by interacting non-covalently with graphene layers Chemicals (Schlierf et al., 2013). They stabilize graphene suspensions by Copper (II) phthalocyanine (CuPc, >95%, Alfa Aesar, MW intercalation between the sonically-destabilized basal planes, 576.07 g/mol, 11 wt.% Cu), 5,10,15,20-tetraphenyl-21H,23H- generating 3D systems in solution and hybrid systems in the porphine copper (II) (CuTPP, Sigma Aldrich, MW 676.27 II solid-state. However, it is interesting that, when it comes to g/mol, 9.4 wt.% Cu), copper nitrate [CuNit, Cu (NO3)2.xH2O, metal-containing dyes, such as copper phthalocyanine (CuPc) Puratronic, 99.999% metals basis, Alfa Aesar, MW 187.55 for example, most work related to the chemical synthesis g/mol (anhydrous)], N,N-dimethylformamide (DMF, >99.8%, of functional CuPc/carbon composites involve graphite oxide Alfa Aesar), 1-methyl-2-pyrrolidone (NMP, ≥99.8%, Alfa Aesar), (Chunder et al., 2010; Mensing et al., 2012; Mukherjee et al., sodium borohydride (NaBH4, ≥98%, Sigma Aldrich), graphite 2017) and high surface area, functionalized carbons (Ding et al., powder (NG, natural, high purity 200 mesh, 99.9999% metal 2012; Goenaga et al., 2014; Reis et al., 2014). There is to our basis, ultra-superior purity, Alfa Aesar) were used without knowledge no example of direct chemical deposition of CuPc further puriﬁcation. on low surface area, bare hydrophobic graphite via non-covalent interactions. Besides, the reported carbon-supported CuPc are Synthesis Using High Power Sonication either used as such, i.e., with no further transformation of the High purity graphite (200 ± 2 mg) was dispersed in 200 mL of immobilized CuPc complex (Pakapongpan et al., 2014; Reis et al., DMF and sonicated using a Bandelin HD2200 probe sonicator 2014; Bian et al., 2020), or after pyrolysis at high temperatures (200 W, 20 kHz), at 50 or 20% of its maximum power, during to modify the carbon support (Ding et al., 2012; Goenaga et al., a time t0 = 5 min. The Cu precursor was then added (181 mg 2014). Their main applications are electrochemistry (Ding et al., for CuPc, 213 mg for CuTPP and 59 mg for copper nitrate, 20 2012; Goenaga et al., 2014; Pakapongpan et al., 2014; Reis et al., mg/0.315 mmol/1.6 × 10−3 M Cu, Cu/NG = 0.10w./w., i.e., 2014; Bian et al., 2020) and photocatalysis (Mukherjee et al., Cu/(Cu+NG) = 9.1% w./w.), after which the mixture was further 2017). When associated with other active supports, CuPc are also sonicated for a time t1 = 5 or 35 min. The solid was recovered by used for catalytic oxidations (Raja and Ratnasamy, 1996; Sorokin, hot ﬁltration (ﬁnal synthesis temperature ∼46–67◦C) and dried 2013) and as co-catalyst for photoelectrochemical water splitting in air for 16–24h at 100◦C. For copper nitrate, one synthesis was (Li et al., 2019). However, there is, to our knowledge, no example performed in the presence of sodium borohydride, as previously of the use of CuPc as a precursor to a catalytically active Cu or described (Michel et al., 2019). In this case, a given amount of −2 CuO phase (Gawande et al., 2016). NaBH4 (119 mg/3.15 mmol/1.6 × 10 M, NaBH4/Cu = 10) was
Frontiers in Chemistry | www.frontiersin.org 2 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine added before recovery of the solid and the mixture was further X-ray Diffraction (XRD) ◦ sonicated for a time t2 = 5 min. Final temperature was 82 C. X-ray Diﬀraction (XRD) patterns of [email protected] composites were The solid was then recovered by hot ﬁltration and dried in air collected on a Bruker D8 Advance theta-theta diﬀractometer for 24h at 100◦C. After cooling down to 22◦C, the sample was (Cu Kα radiation, λ = 0.154nm), equipped with a LynxEye washed with deionised water (2∗200mL) and dried in air for 24h detector and operating at 40 kV and 40mA. The datasets were at 100◦C. acquired in step-scan mode over the 25–58◦ 2θ range, using a step One CuPc/graphite composite was subsequently calcined interval of 0.0132◦ and a counting time of 1s per step. Samples in 10% O2/He under the following conditions: 100 mL/min, were prepared by weighing out 50 mg of catalyst and pressing at 5◦C/min, 400◦C, 30 min. Final composites are denoted X%Cu about 6,300 kg/cm2 (Eurolabo press, 5 t), to get ﬂat and smooth precursor/graphite[Y], where X% stands for the copper weight pellets which were then deposited on round-shaped glass plates. content, Cu precursor stands for the copper precursor used Average size of CuO crystallites (dCuO) was determined by the (CuPc, CuTPP, or Cu(NO3)2) and Y stands for the main Scherrer equation, using the full widths at half-maximum (β = synthesis parameters, i.e., sonication power, contact time, use π× FWHM/180) of the CuO (002) and (111) reﬂections at 2θ = ◦ of NaBH4, ﬁnal temperature in Celsius of the heat treatment. 35.5 and 38.7 , respectively: Six composites were synthesized: CuPc/graphite[50%/5 min], CuPc/graphite[50%/5 min/400], CuPc/graphite[20%/35 min], 0.9 λ 0.9 λ CuTPP/graphite[20%/35 min], CuNit/graphite[20%/35 min], dCuO = ( + )/2 βCuO(002)cosθCuO(002) βCuO(111) cos θCuO(111) CuNit/graphite[50%/5 min/NaBH4]. Synthesis Using Low Power Sonication Slight diﬀerences in peak positions were observed [e.g., 26.3 ± ◦ This procedure was previously described (Vigneron et al., 2014). 0.4 for C(002)]. They were attributed to slight diﬀerences in High purity graphite (100 ± 1 mg) was dispersed in 55 mL of the z and corrected by adjusting the position of the C(002) peak ◦ DMF and sonicated using a Bandelin HD2200 probe sonicator maximum at 26.5 . (200W, 20kHz), at 20% of its maximum power, during a time t0 = 5 min. The beaker containing the mixture was then transferred Fourier Transform Infrared (FTIR) to a sonication bath (Elma, ElmasonicOne, 30 W, 35 kHz). The Fourier transform infrared (FTIR) spectra were recorded by Attenuated Total Reﬂectance with a Thermo Fisher Nicolet iS10 bath contained 200mL of water. The beaker was placed and −1 maintained in a speciﬁc position within this water bath to ensure spectrometer in the 525–4,000 cm range. Powders (few mg) are × repeatability of the preparation (Vigneron et al., 2014). The placed directly on the 2 2 mm diamond window and cover the mixture was allowed to cool down to room temperature (about whole surface. ◦ 22 C) before the Cu precursor was added (92 mg for CuPc Thermogravimetric Analysis (TGA) and 107 mg for CuTPP, 10 mg/0.16 mmol/0.8 × 10−3 M Cu, Thermogravimetric analysis (TGA) was performed on a TGA Cu/NG = 0.10 w./w., i.e., Cu/(Cu+NG) = 9.1% w./w., unless Q5000 from TA Instruments. The powder sample (1.0 ± 0.1 mg) otherwise mentioned). The sonication bath was then turned on ◦ was placed in a Pt pan, which was then heated to 1,000 C at and the mixture allowed to sonicate for a time t = 60, 120, or ◦ 1 10 C/min under ﬂowing air (25 mL/min). Evolution of weight 240 min. The solid was recovered by hot ﬁltration (ﬁnal synthesis loss was monitored by the TA Qseries software. temperature ∼53–71◦C) using nylon membrane ﬁlters (0.45 µm pore size) and dried in air for 21h at 100◦C. Temperature Programmed Reduction (TPR) Two Cu precursor/graphite composites were subsequently Temperature programmed reduction (TPR) was carried out on calcined in static air using a muﬄe furnace under the following an AutochemII Chemisorption apparatus from Micromeritics ◦ ◦ conditions: 10 C/min, 450 C, 2 h. Final composites are denoted equipped with a thermal conductivity detector. The sample X%Cu precursor/graphite[Y], where X% stands for the copper (23mg) was loaded in a quartz tube and heated to 900◦C under a weight content, Cu precursor stands for the copper precursor ﬂowing mixture of 10% H2/Ar (5 mL/min) using a temperature used (CuPc or CuTPP) and Y stands for the main synthesis ramp of 5◦C/min. parameters, i.e., type of sonication (bath), contact time, initial Cu/NG ratio when it is decreased to 1 wt.%, solvent when it Scanning Electron Microscopy (SEM) is changed to NMP, ﬁnal temperature in Celsius of the heat Scanning Electron Microscopy (SEM) was carried out on a Zeiss treatment. Eleven composites were synthesized, as detailed in Gemini SEM 500 system at 10 kV using a working distance (WD) Table 1. of 13.3mm and an aperture (AP) of 30 µm, unless otherwise mentioned. Two detectors were used alternatively: an in lense Elemental Analysis (ICP) secondary electron detector (In Lens) for best imaging resolution Elemental analysis (ICP) of the composites was performed and a Everhart-Thornley detector (SE) for the detection of by Inductively Coupled Plasma Optical Emission Spectroscopy secondary electrons providing both topography and chemical (ICP-OES, Varian 720ES) at IPHC/CNRS UMR7178 (France). contrast, with the lightest elements (C) appearing darker than Deposition yields (deposition eﬃciencies) are deﬁned as the ratio the heaviest elements (Cu). An EDXS SDD probe (30 nm2) between the copper content determined by ICP and the initial conﬁrmed that C, Cu, and O were the only elements present Cu/(Cu+NG) value introduced in the synthesis mixture. in the composites and that the white spots were indeed copper
Frontiers in Chemistry | www.frontiersin.org 3 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
TABLE 1 | Main sonication parameters used for the synthesis of graphite-immobilized copper complexes, resulting Cu content and thermal stability of the synthesized composites.
◦ c Entry Composite Sonication conditions Cu content Targeted Cu Deposition T1/2 ( C) (wt.%)a content efﬁciency (wt.%) (%)b Power (W) Time
1 CuPc/graphite[50%/5 min] 100 5′-5′ 3.5 5.2 67 n.a. 2 CuPc/graphite[20%/35 min] 40 5′-35′ 4.6 5.2 88 647 3 CuPc/graphite[bath/60 min] 30 (bath) 5′-60′ 6.4 5.2 100f 633 4 CuPc/graphite[bath/120 min] 30 (bath) 5′-120′ 5.5 5.2 100f 658 5 CuPc/graphite[bath/60 min/1%]d 30 (bath) 5′-60′ 0.69 0.94 73 742 6 CuPc/graphite[bath/120 min/1%]d 30 (bath) 5′-120′ 0.76 0.94 81 742 7 CuTPP/graphite[20%/35 min] 40 5′-35′ 5.2 4.9 100 668 8 CuTPP/graphite[bath/120 min] 30 (bath) 5′-120′ 3.9 4.9 80 730 9 CuTPP/graphite[bath/240 min] 30 (bath) 5′-240′ 3.0 4.9 61 735 10 CuTPP/graphite[bath/240 min/NMP]e 30 (bath) 5′-240′ 0.62 4.9 13 757 11 CuTPP/graphite[bath/120 min/1%]c 30 (bath) 5′-120′ 0.16 0.89 18 774 12 CuTPP/graphite[bath/240 min/1%/NMP]d,e 30 (bath) 5′-240′ 0.06 0.89 7 785 13 CuNit/graphite[20%/35 min] 40 5′-35′ 0.02 9.1 0.2 753 ′ ′ 14 CuNit/graphite[50%/5 min/NaBH4] 100 5 -5 0.7 9.1 8 n.a. 15 CuPc/graphite[50%/5 min/400] 100 5′-5′ 7.8 - - n.a. 16 CuPc/graphite[bath/60 min/1%/450]d 30 (bath) 5′-60′ 0.77 - - n.a. 17 CuTPP/graphite[bath/240 min/1%/NMP/450]d,e 30 (bath) 5′-240′ 0.06 - - n.a. aBased on ICP measurements (a relative standard deviation of ±5% applies to the reported values), except for entries 15–17. For the last 3 entries, the Cu content is estimated by attributing the weight loss measured after calcination to carbonaceous material (Michel et al., 2019). bDeposition efﬁciency is the ratio, between the real Cu content as measured by ICP and the targeted Cu content based on the Cuprec/(Cuprec+graphite) weight ratio initially present in the synthesis mixture, i.e., 5.2, 4.9, and 9.1 wt.% for CuPc, CuTPP, and CuNit-based composites, respectively. cTGA-derived temperature of half decomposition of graphite deﬁned as the maximum of the weight loss vs. temperature derivative above 500◦C (derivatives of the curves presented in Figure 1, not shown). It corresponds to the temperature at which 50% of graphite is oxidized. dSynthesis using an initial Cu/graphite ratio of 1 wt.%. eUse of NMP instead of DMF as synthesis solvent. f The excess copper found by ICP is attributed to loss of unreacted graphite on the walls of the beaker upon slight evaporation of the DMF solvent at the extended reaction times. oxides. The powder samples were pressed on a sample holder oxygen is exactly half of the consumption of CO. Hence the decorated with carbon tape before analysis. reaction strictly follows the stoichiometry of the CO oxidation reaction (CO + ½ O2 CO2) for both catalysts, which makes the formation of CO via the Boudouart reaction (reduction of Catalytic Evaluation the CO2 product by the graphitic matrix) quite unlikely, even Catalytic evaluation was performed in a fully automated at high conversion levels. Besides, the CO conversion proﬁles in (CETRIB SARL, Andlau, France) ﬁxed-bed ﬂow reactor (i.d. PROX show no evidence for the occurrence of the water gas shift 10mm) loaded with 26mg of composite (0.26–2.5mg CuO/3.2– reaction (WGS) or the reverse water gas shift reaction (RWGS) 32 µmol Cu). The gas mixtures balanced in He, i.e., 1% CO/1% (Ivanova et al., 2010). O2 for CO oxidation and 1% CO/1% O2/24% H2 for the oxidation of CO in the presence of H2 (PROX), were introduced RESULTS AND DISCUSSION at a total ﬂow rate of 100 mL/min (1 atm, GHSV ∼ 15,000 h−1). The composite was heated at 1◦C/min from 20 to 300◦C Incorporation of Copper and then cooled down at the same rate. The O2 and CO signals Sonicating a bulk graphite suspension in the presence of an were monitored using an on-line Compact Gas Chromatograph aromatic copper precursor does result in the atomic scale mixing (Interscience, Belgium) equipped with a thermal conductivity of copper and graphite in the dried composite. Table 1 shows detector. O2 and CO conversions were determined on the basis that up to 7.8% of copper can be introduced into bulk graphite of external calibration. Selectivity to CO2 is deﬁned as the ratio (entry 15) under our conditions and that the copper content is between the number of mole of O2 used to convert CO (i.e., dependent on sonication conditions, the copper complex and the half of the number of mole of CO converted) over the total post-synthesis work-up. number of mole of O2 converted. It is calculated as follows: SCO2 = conv(CO)/2/conv(O2), where conv(CO) and conv(O2) are the Effect of Sonication Conditions conversions of CO and O2, respectively. It is noted that, in the For CuPc, higher incorporation beneﬁts from a longer contact H2-free CO oxidation reaction, the monitored consumption of time at reduced sonication power, rather than high sonication
Frontiers in Chemistry | www.frontiersin.org 4 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine power for a short time. Table 1 (entries 1–3) indeed shows graphitic structure than the 3D CuTPP complex which exhibits that the copper content of the dried composite measured by a larger cross-section. In addition, the planar CuPc complex is ICP steadily increases when the time of sonication is increased expected to more strongly interact with a graphene surface than from 5–35 to 60min (while the sonication power is at the same CuTPP for which stacking of the porphine ring can be seriously time decreased from 100–40 to 30W). This highlights the dual hindered by the out-of-plane phenyl groups (Scheme 1). The role of the sonication energy on the composite formation. On introduction of CuPc thus requires milder exfoliation conditions one hand, sonication is indeed intended to destabilize graphene than the introduction of CuTPP. stacks by weakening π-π interactions between graphene layers, To preliminary understand the role of the ligands in the to enhance diﬀusion of the solvated CuPc in-between graphene incorporation of copper, controlled experiments were conducted layers and thus to maximize the accessible surface for CuPc- by sonicating the bulk graphite suspension in the presence of graphene stacking. On the other hand, it weakens the CuPc- an uncomplexed copper salt, namely copper nitrate (entries 13 graphene interaction that can possibly be engineered under these and 14). None of the conditions tested led to any signiﬁcant conditions. Hence it is expected to ﬁnd an optimum in the incorporation of copper in the dried composite. The direct time/power couple used for sonication to reach full incorporation interaction between Cu2+ and graphene is expected to be of the complex. Further extending the sonication time to 120 min pretty weak, as multivalent cation-π interactions are known at low power (30W, entry 4) leads to an apparent decrease in the to be much weaker than extended π-π interactions (Neel copper content. Nevertheless, the maximum Cu content expected et al., 2017). It is thus consistent with the low Cu content in an as-synthesized CuPc/graphite composite starting from observed in entry 13. On the other hand, conditions of entry 14 Cu/graphite = 10 wt.% is 5.2 wt.%. Indeed, the whole complex (addition of sodium borohydride to the nitrate/graphite mixture) (including the Pc ligand) is present in the dried composite, as will previously allowed us to incorporate signiﬁcant amounts of be shown in section Characteristics of the Interaction of Copper cobalt in graphitic matrices, using hydrolyzed NaBH4 derivatives With the Graphitic Matrix. Besides, the Cu metal center accounts as linkers (Michel et al., 2019). The much lower copper content for only 11 wt.% of the CuPc complex, so that for Cu/graphite obtained here suggests that the linkage between copper/copper = 10 wt.%, Cu/(CuPc+graphite) = 5.2 wt.%. Hence, the ICP- oxides and graphene is not as eﬃcient, as will be discussed in derived Cu contents shown for entries 3 and 4 both suggest section Characteristics of the Interaction of Copper With the full copper deposition, in agreement with the colorless ﬁltrates Graphitic Matrix. observed in these syntheses. Hence, in the case of copper, eﬃcient incorporation in a For CuTPP, full deposition has only been achieved with high graphitic matrix relies on the presence of complexing ligands sonication power (entry 7). Mild sonication leads to about 80% with aromatic properties, which exhibit potential for π stacking CuTPP deposition in 2 h (entry 8), considering the maximum with the aromatic graphene surface. Cu content of 4.9 wt.% expected upon full CuTPP deposition (Cu content in CuTPP is 9.4 wt.%). Further extending the Effect of Solvent and Copper Concentration sonication time (entry 9) leads to a further decrease in Cu N-methyl pyrrolidone (NMP) was previously identiﬁed as a more incorporation eﬃciency to about 60%. Thus, in the case of eﬃcient solvent than DMF for the sonication-assisted liquid- CuTPP, potentially increasing diﬀusion of the solvated complex phase exfoliation of graphite (Coleman, 2013). By comparing in-between graphene layers does not result in enhanced Cu entries 9 and 10, it appears that replacing the DMF solvent by incorporation. This is attributed to a poor porphine/graphene NMP in our synthesis actually results in a net decrease in the interaction, as compared with the CuPc/graphene interaction. deposition of Cu from 60 to about 12%. This suggests that the Indeed, the four freely rotating phenyl groups of the CuTPP more exfoliating NMP molecule competes more severely with complex are expected to inhibit eﬃcient stacking of the porphine CuTPP for the interaction with the graphene surface. complex to the graphene surface (Scheme 1). Sonication will thus Decreasing the Cu/graphite ratio from 10 to 1 wt.% results in easily break the porphine/graphene stacks, and more and more so a general decrease in deposition eﬃciency from 100% (entries with increasing time. 3 and 4) down to 73 and 81% for CuPc (entries 5 and 6, respectively), and from 80 and 61% (entries 8 and 9, respectively) Effect of Copper Precursor down to 18 and 7% for CuTPP (entries 11 and 12, respectively). Comparing entries 4 and 8, it appears that the incorporation of Two phenomena may explain these results. First, a decrease in the CuTPP complex is less eﬃcient than that of CuPc, with only the concentration of the copper complex decreases the osmotic 80% CuTPP deposition observed under sonication conditions pressure within the graphitic structure, hence the diﬀusion of that lead to full CuPc deposition. On the other hand, comparing the complex within the structure and the possibility for the entries 2 and 7, it appears that deposition of the CuTPP complex copper complex to compete with interlayer stacking. Second, under high power sonication is more eﬃcient than that of CuPc, the lower concentration also increases the competition between with full vs. 90% deposition respectively. This is attributed to the copper complex and the solvent for interacting with the diﬀerences in the geometry of the complexes. CuPc is indeed graphene surface, which is not in favor of the complex. Hence much more planar than CuTPP that contains 4 freely rotating the particularly low Cu content of entry 12 is the result of a phenyl groups regularly distributed around the porphine ring. combination of low concentration of the copper complex, use of Hence, it is expected that the 2D CuPc complex will diﬀuse the highly exfoliating solvent NMP and the non-planar nature of much more eﬃciently within the sonically-destabilized lamellar the CuTPP complex.
Frontiers in Chemistry | www.frontiersin.org 5 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
SCHEME 1 | Schematic representation of the possible interactions of CuPc and CuTPP complexes with a sonically-destabilized graphitic matrix.
Characteristics of the Interaction of supports ﬁrm immobilization of the complex onto graphene. Copper With the Graphitic Matrix In particular, for CuPc/graphite, oxidation of graphite directly TGA follows degradation of the complex, which clearly indicates Impact of complex immobilization the presence of a strong interaction between the planar Pc Oxidation of the composite in air is driven by the complex, which complex and the graphenic surface, most likely in the form shifts the oxidation of graphite at much lower temperature, as of highly delocalized π interactions. The small, yet signiﬁcant, shown by the following TGA study (Figure 1). TGA proﬁles temperature interval between oxidation of TPP and oxidation of the composites prepared by high power sonication (entries of graphite in CuTPP/graphite is consistent with the weaker 2 and 7) are shown in Figure 1A (plain lines). They both interaction between the 2 components, due to the non-planar exhibit 2 distinct weight losses, which are attributed to oxidative nature of the TPP complex. Nevertheless, both complexes degradation of the complex (lower temperature) and oxidation induce a drastic decrease in the oxidation temperature of the graphitic matrix (>100◦C). By comparison, stability of graphite of the graphitic matrix (higher temperature), by comparison with ◦ TGA proﬁles of free complexes (dotted lines) and bare sonicated (750 C) is only marginally aﬀected by the presence of Cu in graphite (black line). In both composites, the temperature of 0.02%CuNit/graphite (entry 13), likely due (1) to the absence of degradation of the immobilized complex is close to that of any strong interaction between Cu and graphite and (2) to the the free complex. On the other hand, the degradation of the small Cu content. graphenic component occurs at much lower temperature than the oxidation of bare graphite. Temperature of half oxidation Impact of complex loading ◦ of graphite (785 C in graphite sonicated in the absence of The impact of the complex loading on the oxidative thermal ◦ copper compounds) is signiﬁcantly decreased (Table 1),to668 C stability of the graphenic component has been studied for both ◦ for 5.2%CuTPP/graphite and to 647 C for 4.6%CuPc/graphite. CuPc/graphite (Figure 1B) and CuTPP/graphite (Figure 1C) It suggests that the oxidation of the graphitic matrix is composites obtained by mild sonication. For CuPc/graphite, induced by oxidative degradation of the complex, which further high loadings (plain lines, entries 3 and 4, 6.4% and 5.5%
Frontiers in Chemistry | www.frontiersin.org 6 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 1 | TGA proﬁles of high power sonication- (A), CuPc- (B), CuTPP- (C) derived composites, including sonicated graphite (50%/DMF/30 min, black line) and in (A), 0.02%CuNit/graphite[20%/35 min] (plain red line), 4.6%CuPc/graphite[20%/35 min] (plain blue line), copper phthalocyanine (dotted blue line), 5.2%CuTPP/graphite[20%/35 min] (plain green line), copper tetraphenylporphine (dotted green line). In (B): 6.4%CuPc/graphite[bath/60 min] (plain light blue line), 0.69%CuPc/graphite[bath/60 min/1%] (dotted light blue line), 5.5%CuPc/graphite[bath/120 min] (plain dark blue line), 0.76%CuPc/graphite[bath/120 min/1%] (dotted dark blue line). In (C): 3.9%CuTPP/graphite[bath/120 min] (plain light green line), 0.16%CuTPP/graphite[bath/120 min/1%] (dotted light green line), 0.62%CuTPP/graphite [bath/240 min/NMP] (plain dark green line), 0.06%CuTPP/graphite[bath/240 min/1%/NMP] (dotted dark green line), 3.0%CuTPP/graphite[bath/240 min] (orange line). (D) Evolution of graphite half-oxidation temperatures as a function of Cu content for CuPc- (blue diamonds) and CuTPP- (green squares) derived composites prepared with bath sonication, as derived from Figures 1B,C, respectively. Black-lined symbols indicate data from high power sonication (Figure 1A).
Cu, respectively) clearly aﬀect the oxidation of the graphenic with increasing CuPc loading thus results in the disappearance of component much more than low loadings (dotted lines, entries the temperature interval (plateau) between the degradation of the 5 and 6, 0.69% and 0.76% Cu, respectively). The temperature complex and the oxidation of graphite. It is noted that the extent of half-degradation of graphite indeed decreases from 742◦C for of the weight loss between 400 and 500◦C related to degradation the low loaded composites to below 658◦C for the highly loaded of the metal complex is much more pronounced for the highly composites (Table 1). On the other hand, the degradation of the loaded composites, which validates the interpretation. Pc complex, which starts at about 400◦C in all cases, is unaﬀected Similar conclusions can be drawn for the CuTPP/graphite by its immobilization within the composite and its loading in the composites: the weight loss attributed to degradation of the composite. The decrease in graphite half-oxidation temperature CuTPP is larger for the highly loaded composites and more
Frontiers in Chemistry | www.frontiersin.org 7 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 2 | Full range (A) and 500–1,700 cm−1 range (B) FTIR spectra of graphite (black line), copper phthalocyanine (gray line), 3.5%CuPc/graphite[50%/5 min]
(blue line), 0.7%CuNit/graphite[50%/5 min/NaBH4] (plain red line), and 7.5%CoNit/graphite[50%/5 min/NaBH4](Michel et al., 2019) (dotted red line). importantly, high CuTPP loadings (entries 8 and 9, 3.9% and Finally, by adding to the graph data from the composites 3.0% Cu, respectively) destabilize the graphenic component more resulting from high power sonication and derived from than low CuTPP loadings (entries 10–12, 0.62%, 0.16%, and Figure 1A, one can see that the graphite half-oxidation 0.06% Cu, respectively). However, this occurs to a lesser extent as temperature of 5.2%CuTPP/graphite (entry 7) is located at a compared with the CuPc/graphite composites: the temperature of much lower temperature than that expected from the logarithmic half-oxidation of graphite and the temperature interval (plateau) trend. It suggests that high power sonication does enhance between the degradation of the complex and the oxidation of the interaction between CuTPP and graphene, as discussed in graphite are both less impacted by the CuTPP content. The section Eﬀect of Copper Precursor. On the other hand, the point temperature interval actually appears quite independent from the related to 4.6%CuPc/graphite (entry 2) is nicely integrated in the CuTPP loading. This is overall attributed to the lower interaction parabolic trend (Figure 1D), highlighting the similar nature of between the 3D CuTPP complex and graphene as compared with the CuPc composites whatever the sonication protocol used. the planar CuPc complex. It overall shows that the impact of the complex loading is conditioned by the strength of the complex- FTIR graphene interaction: the stronger the interaction, the stronger FTIR spectra of 3.5%CuPc/graphite[50%/5 min] (entry 1) and the impact. 0.7%CuNit/graphite[50%/5 min/NaBH4] (entry 14) are shown in This is conﬁrmed by plotting the temperature of graphite Figure 2. half-oxidation vs. ICP-derived Cu content (Figure 1D). Such CuPc/graphite[50%/5 min] exhibits a well-deﬁned vibrational temperatures are systematically lower for the CuPc vs. CuTPP- pattern in the 500–1,700 cm−1 wavenumber region (Figure 2A) containing composites. The diﬀerence is higher at higher Cu which can unambiguously be attributed to aromatic C-C, C- contents, due to the parabolic decrease of half oxidation N, and C-H vibrations of the phthalocyanine ligand (Seoudi temperatures vs. Cu contents for CuPc/graphite composites et al., 2005), as clearly evidenced by comparison with the instead of the logarithmic decrease observed for CuTPP- FTIR spectrum of the free CuPc complex. This evidences the containing composites. Such diﬀerent variations in graphite half- presence of the complex in the composite. Overall intensity oxidation temperatures as a function of the copper content of the CuPc pattern is lower in the composite than in are consistent with diﬀerences in the strength of interaction the free CuPc. More interestingly, by normalizing the CuPc that the complex develops with the graphene surface. The and CuPc/graphite spectra to in-plane vibrations, and more stronger decrease in graphite half-oxidation temperatures with speciﬁcally to the main C-C and C-N vibrations of isoindole increasing Cu content observed for CuPc-containing composites at 1,325 and 1,285 cm−1, respectively (Figure 2B), C-H out- is consistent with the stronger interaction that the 2D planar of-plane vibrations (728, 752, 870, 896 cm−1) clearly appear complex is able to engineer with the planar graphene surface, less intense in the composite than in the free complex. Besides, as compared with the 3D CuTPP complex which contains four ring deformation (637 cm−1) is lost in the FTIR spectrum freely rotating phenyl groups (Scheme 1). of the composite. Such inhibition of out-of-plane vibrations
Frontiers in Chemistry | www.frontiersin.org 8 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 3 | XRD of 7.8%CuPc/graphite[50%/5 min/400] (A) and sonicated graphite (50%/DMF/30 min, black line), 0.8%CuPc/graphite[bath/60 min/1%/450] (blue line), and 0.06%CuTPP/graphite[bath/240 min/1%/NMP/450] (green line) (B) in the 2θ range of 34 to 40◦, showing CuO reﬂections. is a clear evidence of immobilization of the complex on a Soft Oxidation of Copper surface, and more speciﬁcally of orientation of the Pc complex ICP, TG and FTIR analyses thus all point to eﬃcient copper parallel to the graphitic surface (Basova et al., 2009). FTIR incorporation using the CuPc complex and to a strong thus gives clear indication that the complex is π-stacked with CuPc/graphite interaction. The following sections will focus graphene layers. In this conﬁguration, C-H bonds may indeed on these composites and especially on the most loaded one be involved in an interaction with the graphene surface or (entry 1). The thermo-oxidative stability of the graphitic matrix lost by deprotonation upon interaction with the carbon surface in these composites is however much lower than that of the and Pc breathing is inhibited as a result of these delocalized parent graphite and an appropriate treatment had to be designed π interactions. to oxidize the immobilized complex without oxidizing the For comparison, CuNit/graphite[50%/5 min/NaBH4] exhibits graphitic matrix. a very similar spectrum to that of a cobalt-containing composite prepared under the same conditions. Both spectra are indeed XRD characterized by two broad bands at 1,050 and 1,340 cm−1 The highly loaded CuPc composite (entry 1, 3.5% Cu) was (Figure 2A). They are attributed to asymmetric stretching calcined at limited temperature and time (400◦C/30 min) vibrations of B-O bonds found in borate compounds (νB(4)−O to limit degradation of the graphitic matrix. The resulting and νB(3)−O, respectively) (Jun et al., 1995). It is consistent with composite (entry 15, 7.8% Cu) was analyzed by X-ray diﬀraction ◦ the presence of moieties derived from NaBH4 hydrolysis and (Figure 3A). Strong reﬂections at 35.5 and 38.7 are observed. oxidation in the composite, as previously discussed (Michel et al., They correspond to the (002) and (111) reﬂections, respectively, 2019). It is likely that these species take part in metal deposition of the monoclinic phase of CuO, in agreement with ICDD since virtually no deposition of copper (or other metal) ion is card No. 48-1548 and with the related literature in the ﬁeld observed in the absence of these species (entry 13). Besides, the (Fuentes et al., 2010; Zhu and Diao, 2012; Du et al., 2016). amount of borate species present in the composites seem to The average primary crystalline domain size is calculated to correlate with the metal content, since FTIR spectra normalized be 27 ± 2 nm using the Debye-Scherrer formula. It is noted to the Cu and Co metal contents exhibit B-O vibrations of similar that the low loaded composite calcined at 450◦C for 2 h intensities. The much lower metal deposition observed for Cu (0.8%CuPc/graphite[bath/60 min/1%/450], entry 16) also exhibit (0.7 wt.%, entry 14) vs. Co (7.5 wt.%, Michel et al., 2019) under distinct CuO-related reﬂections at 35.5 and 38.7◦ (Figure 3B). similar synthesis conditions can thus be attributed to diﬀerences On the other hand, no Cu-related reﬂections is found for the in the catalytic properties of the two metals for NaBH4 hydrolysis calcined composite with the lowest Cu content (0.06 wt.%, entry and to diﬀerences in the ability of the two metals to form borate 17) (Figure 3B). compounds from the metals themselves. In this regard, cobalt is a much more eﬃcient catalyst for NaBH4 hydrolysis, which TPR readily involves the formation of cobalt borides and borates The TPR proﬁle of 7.8%CuPc/graphite[50%/5 min/400] (entry (Demirci and Miele, 2010). On the other hand, the formation 15) further shows that CuO is the only copper phase present of such stable copper compounds is not observed (Glavee et al., in the composite (Figure 4). The reduction proﬁle indeed 1994). exhibits 2 main peaks at 228 and 315◦C, which can be
Frontiers in Chemistry | www.frontiersin.org 9 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
that expected from CuO (7.7/63.5∗16 = 1.94 wt.%) in those areas. It is consistent with the occurrence of CuPc adsorption close to the edges (without deep diﬀusion inside the graphitic matrix due to the limited reaction time of 5 min), as shown in Figures 6C,D, which is further supported by the peculiar patterns created by the spatial distribution of CuO over graphite. The in-plane dimensions of graphite ﬂakes are similar to those observed in the copper-free parent graphite submitted to a similar sonication treatment (10–100nm). On the other hand, thinner stacks can be found in the composites before (Figure 6C) and after oxidation, as compared with the Cu-free sonicated parent. It is attributed to insertion of copper phthalocyanine and copper oxides in-between graphite ﬂakes (Figure 5D), which disturbs ordering of graphene layers in the direction normal to the plane.
Copper-Induced Solid-State Exfoliation of Graphite X-ray diﬀractograms of the oxidized composites all exhibit a major and dominating reﬂection at 26.5◦ which can be attributed FIGURE 4 | H2-TPR spectrum of 7.8%CuPc/graphite[50%/5 min/400]. to C(002) reﬂection of graphite and is due to the stacking of graphene layers in the c direction (normal to the plane). By using mass-normalized intensities, one can clearly observe attributed to the reduction of CuO into Cu2O and to the broadening of the peak in the composites, as compared with reduction of Cu2O into Cu, respectively (Song et al., 2013; bare graphite (treated under high power sonication conditions Silva et al., 2015; Ma et al., 2018). Both peaks exhibit similar at 50% power in DMF for 30min in the absence of any copper intensities. Given the stoichiometry of the sequential reduction precursor), while the overall intensity of the peak remains similar. (2CuO + H2→Cu2O + H2O and Cu2O + H2→2Cu + The full width at half-maximum appears indeed systematically H2O), the same amount of hydrogen is needed to reduce larger in Cu-containing composites than in bare sonicated CuO into Cu2O and then the produced Cu2O into Cu. graphite (Figure 7A). According to the Debye-Scherrer law, Hence, it can be concluded that fully oxidized CuIIO is this indicates that the average thickness of graphene stacks is the sole phase of Cu that is present in the composite. smaller in the composites. It suggests that CuO particles and The thin, well-deﬁned peaks indicate high crystallinity of the agglomerates may act as inorganic exfoliating agents, thereby copper oxide phase, in agreement with XRD results (section decreasing the average degree of graphene stacking in the dried XRD) (Michel et al., 2019). Finally, the position of the low composite. Using the Debye-Scherrer law, this decrease can temperature reduction peak occurs at lower temperature than be estimated to be about 36 ± 3%. 30 nm- and 33 nm-thick that usually found for bulk CuO (280◦C, Silva et al., 2015). stacks are indeed calculated for the 0.8%CuPc/graphite (entry It is attributed to the reducing character of the carbonaceous 16) and 0.06%CuTPP/graphite (entry 17) oxidized composites, support which could facilitate the reduction of the supported respectively, instead of 49nm for bare graphite. Hence, although cupric oxide. the exfoliation of graphite is somehow limited, as compared with the level of exfoliation achieved in the liquid phase with SEM speciﬁcally designed techniques (Coleman, 2013), the thickness This material was further analyzed by Scanning Electron of graphite ﬂakes may still be decreased by about one third Microscopy (Figure 5). Quite high coverage of the graphitic on average in the solid state. This is in line with the low support by CuO is observed at the micrometric scale amount of CuO in these composites and the use of standard (Figures 5A,B). CuO mostly appears in the form of drying (instead of freeze-drying) prior to the soft oxidation. aggregates/chains of 100 nm particles randomly distributed Interestingly, the highly loaded 7.8%CuO/graphite composite over graphite ﬂakes (Figures 5C–F). In these areas, the Cu (entry 15) exhibits a smaller broadening of the intensity- content determined by EDX (7.7 wt.%) is strikingly similar to normalized C(002) reﬂection (Figure 7B). It is attributed to the overall Cu content determined by ICP (7.8 wt.%). Huge weaker diﬀusion of the CuPc complex within the graphitic CuO particles (500 nm−1 µm) are also present. Graphite edges matrix due to limited reaction time (5 min). Hence broadening appear strongly damaged in the composites (Figures 5C,E), as of the peak and the corresponding general mild exfoliation compared with the straight edges present in the parent graphite of graphite obtained in the solid state by mere incorporation (Figures 6A,B). This is attributed to local oxidation of graphene of copper oxide nanoparticles are mainly determined by the layers edges upon oxidation of CuPc as indicated by the high time of sonication and in turn diﬀusion of the complex local O content (3.5 wt.%) found by EDX, which largely exceeds within the graphitic matrix, rather than bare Cu content. Still,
Frontiers in Chemistry | www.frontiersin.org 10 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 5 | SEM images of 7.8%CuPc/graphite[50%/5 min/400] from SE (A–D) and InLens detectors (E,F), showing CuO-decorated graphite ﬂakes (A), large CuO particles deposited on graphene (B), decoration of graphene edges with smaller CuO particles (C), intercalation of CuO NPs (D), damaged graphene edges (E), and CuO aggregates/chains (F). thinner graphitic stacks may locally be observed in uncalcined Catalysis 3.5%CuPc/graphite (Figure 6C) as compared with bare sonicated Oxidized CuPc/graphite (entry 15, 7.8% Cu) and CuNit/graphite graphite (Figure 6A), indicating that CuPc platelets may indeed (entry 14, 0.7% Cu) were tested for the oxidation of CO both in intercalate in-between graphene layers and break the stacking of the absence (open symbols) and in the presence (plain symbols) the ﬂakes. of hydrogen (Figures 8A–F).
Frontiers in Chemistry | www.frontiersin.org 11 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 6 | SEM images taken at 12 kV from InLens detectors of the parent graphite sonicated at 50% power in DMF for 30 min (A,B) (WD = 11.8 mm, AP = 60 µm) and of 3.5%CuPc/graphite[50%/5 min] (C,D) (WD = 11.3 mm, AP = 30 µm), showing thick stacks of graphene layers (A), straight, undamaged edges (B), thinner graphitic stacks (C), and deposited and intercalated CuPc platelets (D).
FIGURE 7 | (A) XRD of sonicated graphite (50%/DMF/30min, black line), 0.8%CuPc/graphite[bath/60 min/1%/450] (blue line) and 0.06%CuTPP/graphite[bath/240 min/1%/NMP/450] (green line) in the 2θ range of 26 to 27◦, showing the main C (002) reﬂection of graphite. (B) XRD of sonicated graphite (black line) and CuPc/graphite[50%/5 min/400] (blue line).
Frontiers in Chemistry | www.frontiersin.org 12 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
FIGURE 8 | Oxidation catalysis. CO conversions (A), CO oxidation rates (B), oxygen conversions (C), oxygen conversion rates (D), selectivity to CO2 vs. temperature (E), and vs. oxygen conversion (F) observed over 7.8%CuPc/graphite[50%/5 min/400] (blue diamonds) and 0.7%CuNit/graphite[50%/5 min/NaBH4] (red squares) in the CO+O2 (open symbols), CO+O2+H2 (full symbols), and H2+O2 (circles) gas-phase reactions. Black lines show the performance of bare graphite. Black line in (C) is for the H2+O2 reaction.
Frontiers in Chemistry | www.frontiersin.org 13 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
Performance of CuPc/graphite[50%/5 min/400] orders of magnitude higher O2 conversion rates observed under Higher CO conversions are achieved at any given temperature, CO-free conditions over the low loaded catalyst (Figure 8D, plain under either of the conditions, by the oxidized CuPc/graphene red circles), which indicate that the low loaded composite is a rather than the nitrate-derived composite (Figure 8A). This is very eﬃcient hydrogen oxidation catalyst. Although its overall essentially attributed to the much higher copper content of activity is signiﬁcantly inhibited by the presence of CO, it retains the Pc-derived catalyst, since mass-normalized CO oxidation its strong hydrogen oxidation character and thus preferentially rates of both composites (Figure 8B) under H2-free conditions oxidizes H2 under competitive conditions (PROX). Under these (open symbols) are much closer. In the presence of hydrogen, conditions, the catalytic properties of the nitrate-derived catalyst oxidized CuPc/graphite exhibits similar CO conversions up to actually resemble those of bare graphite, in terms of both CO about 210◦C, at which point the CO conversion decreases, conversion (Figure 8A) and selectivity (Figure 8D) levels. The due to unfavorable competition with hydrogen (CO/H2 = oxidizing properties of copper thus appear mute/silent, turned 1/24) for the limited amount of oxygen present in the oﬀ by the presence of hydrogen. We speculate that this may feed (1%). This is generally observed in metal- (Laveille be due to the particularly low amount of copper present on et al., 2016) and oxide- (Michel et al., 2019) catalyzed CO the catalyst (0.7 wt.%) with regard to the reducing properties PROX. Nevertheless, hydrogen has virtually no impact on low of graphite and to the reactivity of the graphene surface toward temperature CO oxidation rates over oxidized CuPc/graphite. H2/O2 mixtures. Oxygen conversions appear similar as well, up to 180◦C The catalytic properties of the Pc-derived composite (Figure 8C), which means that the amount of oxygen converted seem on the other hand essentially controlled by the in the oxidation of CO under hydrogen-free conditions CuO phase. Intrinsic activities for CO oxidation (0.12 ◦ (CO+O2) is similar to the total amount of oxygen used mmolCO/gCuO/s at 200 C) are indeed similar to those for oxidizing both CO and H2 under PROX conditions previously reported over CuO/γ-Al2O3 under optimized (CO+O2+H2). Hence only a minor amount of hydrogen is pre-treatment conditions (0.091 mmolCO/gCuO/s) (Wan et al., converted below 180◦C, as shown by the high selectivity to 2008). The intrinsic activity of oxidized CuPc/graphite is ◦ CO2 which remains above 80% up to 180 C (Figure 8E) and however signiﬁcantly higher than that of air calcined CuO/γ- up to 15% O2 conversion (Figure 8F). Hydrogen starts to Al2O3 (0.02 mmolCO/gCuO/s), highlighting the relevance be signiﬁcantly converted above 180◦C, as indicated by both of the sonication-induced decoration of graphite with the higher oxygen conversions observed from 180◦C under copper phthalocyanine in the preparation of copper oxide PROX conditions (plain diamonds) as compared with the oxidation catalysts. hydrogen-free conditions (open diamonds), and the decreasing selectivity to CO2 with both temperature (Figure 8E) and oxygen conversion levels (Figure 8F). In the absence of CO in CONCLUSIONS the feed (H2+O2 feed, blue circles), oxygen conversions are similar to those obtained in the CO+O2 and the CO+O2+H2 The copper phthalocyanine metal complex was successfully conditions up to 180◦C; they remain close to those observed deposited on unfunctionalized, hydrophobic, bulk graphite and ◦ in CO+O2+H2 conditions above 180 C. This suggests that used as precursor to a catalytically active CuO phase for CO the overall activity of oxidized CuPc/graphite is virtually oxidation, with no need for extensive exfoliation of graphite. independent of the reaction conditions. This highly loaded Introduction of CuPc within the graphitic matrix is achieved by a catalyst can independently convert CO (1%) and H2 (24%) liquid phase sonication procedure, using the DMF solvent as soft, at the same rate, but it preferentially oxidizes CO at lower temporary co-exfoliating agent. Immobilization of the complex temperatures under competitive conditions (PROX). This is onto graphene layers is evidenced in the solid state by loss of IR- in marked contrast with what is observed on the low loaded active out-of-plane vibration modes of the Pc ligand. The strong CuNit/graphite catalyst. hydrophobic π-π-based interaction leads to destabilization of the graphitic matrix under oxidative conditions, as shown by Performance of CuNit/graphite [50%/5 min/NaBH4] TGA. Destabilization of the graphitic matrix is directly related While both catalysts exhibit similar CO oxidation rates in the to both the strength of the interaction, as shown by comparison absence of hydrogen (Figure 8B), the nitrate-derived catalyst is with the non-planar CuTPP complex, and the CuPc/graphite much less active toward CO oxidation under PROX conditions ratio. Controlled thermal oxidation of dried [email protected] (Figure 8B, plain squares). Nevertheless, its overall activity is not composites results in mild exfoliation of the graphitic structure. modiﬁed by the presence of hydrogen, as oxygen is converted A limited, yet signiﬁcant degree of exfoliation can indeed be at the same rate under CO+O2 (Figure 8C, open squares) and obtained in the solid state at low Cu content (<1 wt.%), despite CO+O2+H2 (Figure 8C, plain squares) conditions. Besides, O2 the low sonication power used, with composites resulting from conversion rates are only 2 to 3 times lower than those observed extended sonication times. This brings indirect evidence that over the Pc-derived catalyst (under kinetic regime, 100–180◦C exfoliation is initially controlled by the diﬀusion of the complex temperature range in Figure 8D). The main diﬀerence is the within the graphitic matrix. Finally, a relatively highly loaded drastically lower selectivity to CO2, which does not exceed 9.7 wt.%CuO/graphite catalyst for CO oxidation and PROX 10% on the low loaded catalyst regardless of temperature and may be obtained. It is more active than standard CuO/γ- conversion levels (Figures 8E,F). This can be correlated to the Al2O3 catalysts, based on CuO mass-normalized reaction rates,
Frontiers in Chemistry | www.frontiersin.org 14 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine highlighting the potential of this new method for the synthesis of manuscript. All authors contributed to the article and approved oxidation catalysts. the submitted version.
DATA AVAILABILITY STATEMENT FUNDING
The raw data supporting the conclusions of this article can be This work was funded by the French National Research Agency made available by the authors upon request. OH Risque Program (PICATA project, ANR-14-OHRI-0005-01).
AUTHOR CONTRIBUTIONS ACKNOWLEDGMENTS
GC: 9 syntheses using bath sonication, 2 calcinations, and 11 The authors wish to thank ANR for funding, Thierry Dintzer TGA. GG: 3 syntheses using tip sonication, 3 TGA, and 2 (ICPEES/CNRS UMR7515) for SEM images and EDX data, XRD. CR: 2 syntheses using tip sonication, 1 TGA and 4 FTIR. Sécou Sall (ICPEES/CNRS UMR7515) for TPR data, and Fabrice LM: 1 calcination (entry 15), 2 XRD and catalytic evaluation. Vigneron (ICPEES/CNRS UMR7515) for technical support on VC: concept, guidance, project management, and writing of the the catalytic micro-pilot.
REFERENCES Goenaga, G. A., Foister, S., Belapure, A., Byrne, K., Hawks, S., Papandrew, A. B., et al. (2014). Pyrolyzed copper-based catalyst with high oxygen reduction Basova, T. V., Jushina, I. V., Gürek, A. G., Atilla, D., and Ahsen, V. (2009). activity for PEM fuel cell applications. ECS Electrochem. Lett. 3, 68–71. The synthesis and characterization of Cu(II) phthalocyanine bearing doi: 10.1149/2.0071411eel peripheral monoazacrown ethers and a spectral investigation of its ﬁlm Goncalves, G., Marques, P. A. A. P., Granadeiro, C. M., Nogueira, H. I. S., Singh, forming character. Dyes Pigm. 80, 67–72. doi: 10.1016/j.dyepig.2008. M. K., and Grácio, J. (2009). Surface modiﬁcation of graphene nanosheets with 05.002 gold nanoparticles: the role of oxygen moieties at graphene surface on gold Bian, Y., Su, L., Yu, Z., Lv, Z., Chen, H., Zhou, Y., et al. (2020). Graphite/copper nucleation and growth. Chem. Mater. 21, 4796–4802. doi: 10.1021/cm901052s phthalocyanine composite cathode for overcharge protection and gas evolution Hummers, W. S., and Oﬀeman, R. E. (1958). Preparation of graphitic oxide. J. Am. suppression in aluminum-ion batteries at room temperature. Electrochimi. Acta Chem. Soc. 80, 1339–1339. doi: 10.1021/ja01539a017 332:135188. doi: 10.1016/j.electacta.2019.135188 Ivanova, S., Pitchon, V., Petit, C., and Caps, V. (2010). Support eﬀects Cai, M., Thorpe, D., Adamson, D. H., and Schniepp, H. C. (2012). Methods of in the gold-catalyzed PROX reaction. Chem Cat Chem 2, 556–563. graphite exfoliation. J. Mater. Chem. 22, 24992–25002. doi: 10.1039/c2jm34517j doi: 10.1002/cctc.200900302 Caps, V., Arrii, S., Morﬁn, F., Bergeret, G., and Rousset, J.-L. (2008). Jun, L., Shuping, X., and Shiyang, G. (1995). FT-IR and Raman Structures and associated catalytic properties of well-deﬁned nanoparticles spectroscopic study of hydrated borates. Spectrochim. Acta 51, 519–532. produced by laser vaporisation of alloy rods. Faraday Discuss. 138, 241–256. doi: 10.1016/0584-8539(94)00183-C doi: 10.1039/B706131E Laveille, P., Biausque, G., Zhu, H., Basset, J.-M., and Caps, V. (2013). A high- Chunder, A., Pal, T., Khondaker, S. I., and Zhai, L. (2010). Reduced graphene throughput study of the redox properties of Nb-Ni oxide catalysts by low oxide/copper phthalocyanine composite and its optoelectrical properties. J. temperature CO oxidation: implications in ethane ODH. Catal. Today 203, 3–9. Phys. Chem. C 114, 15129–15135. doi: 10.1021/jp104587n doi: 10.1016/j.cattod.2012.05.020 Coleman, J. N. (2013). Liquid exfoliation of defect-free graphene. Acc. Chem. Res. Laveille, P., Guillois, K., Tuel, A., Petit, C., Basset, J.-M., and Caps, V. (2016). 46, 14–22. doi: 10.1021/ar300009f Durable PROX catalyst based on gold nanoparticles and hydrophobic silica. Demirci, U. B., and Miele, P. (2010). Cobalt in NaBH4 hydrolysis. Phys. Chem. Chem. Commun. 52, 3179–3182. doi: 10.1039/C5CC09561A Chem. Phys. 12, 14651–14665. doi: 10.1039/c0cp00295j Li, Y., Yang, M., Tian, Z., Luo, N., Li, Y., Zhang, H., et al. (2019). Ding, L., Qiao, J., Dai, X., Zhang, J., Zhang, J., and Tian, B. (2012). Highly Assembly of copper phthalocyanine on TiO2 nanorod arrays as co-catalyst active electrocatalysts for oxygen reduction from carbon-supported copper- for enhanced photoelectrochemical water splitting. Front. Chem. 7:334. phthalocyanine synthesized by high temperature treatment. Int. J. Hydrogen doi: 10.3389/fchem.2019.00334 Energy 37, 14103–14113. doi: 10.1016/j.ijhydene.2012.07.046 Ma, L., Han, D., Ma, H., Liu, L., and Guo, H. (2018). Characterization of highly Dreyer, D. R., Todd, A. D., and Bielawski, C. W. (2014). Harnessing the chemistry dispersed rod- and particle-shaped CuFe19Ox catalysts and their shape eﬀects of graphene oxide. Chem. Soc. Rev. 43, 5288–5301. doi: 10.1039/C4CS00060A on WGS. Catalysts 8:635. doi: 10.3390/catal8120635 Du, X., Huang, J., Feng, Y., and Ding, Y. (2016). Flower-like 3D CuO microsphere Mars, P., and van Krevelen, D. W. (1954). Oxidations carried out by acting as photocatalytic water oxidation catalyst. Chinese J. Catal. 37, 123–134. the means of vanadium oxide catalysts. Chem. Eng. Sci. 3, 41–59. doi: 10.1016/S1872-2067(15)61012-9 doi: 10.1016/S0009-2509(54)80005-4 Freund, H.-J., Meijer, G., Scheﬄer, M., Schlögl, R., and Wolf, M. (2011). CO Mensing, J. P., Kerdcharoen, T., Sriprachuabwong, C., Wisitsoraat, A., oxidation as a prototypical reaction for heterogeneous processes. Angew. Chem. Phokharatkul, D., Lomas, T., et al. (2012). Facile preparation of graphene– Int. Ed. 50, 10064–10094. doi: 10.1002/anie.201101378 metal phthalocyanine hybrid material by electrolytic exfoliation. J. Mater. Fuentes, S., Zárate, R. A., Muñoz, P., and Díaz-Droguett, D. E. (2010). Chem. 22, 17094–17099. doi: 10.1039/c2jm32588h Formation of hierarchical CuO nanowires on a copper surface via a room- Michel, L., Sall, S., Dintzer, T., Robert, C., Demange, A., and Caps, V. (2019). temperature solution-immersion process. J. Chil. Chem. Soc. 55, 147–149. Graphene-supported 2D cobalt oxides for catalytic applications. Faraday doi: 10.4067/S0717-97072010000100034 Discuss. doi: 10.1039/C9FD00110G Gawande, M. B., Goswami, A., Felpin, F.-X., Asefa, T., Huang, X., Silva, R., et al. Mukherjee, M., Ghorai, U. K., Samanta, M., Santra, A., Das, G. P., and (2016). Cu and Cu-based nanoparticles: synthesis and applications in catalysis. Chattopadhyay, K. K. (2017). Graphene wrapped copper phthalocyanine Chem. Rev. 116, 3722–3811. doi: 10.1021/acs.chemrev.5b00482 nanotube: enhanced photocatalytic activity for industrial waste water Glavee, G. N., Klabunde, K. J., Sorensen, C. M., and Hadjipanayis, G. C. (1994). treatment. Appl. Surf. Sci. 418, 156–162. doi: 10.1016/j.apsusc.2017.01.222 Borohydride reduction of nickel and copper ions in aqueous and nonaqueous Neel, A. J., Hilton, M. J., Sigman, M. S., and Toste, F. D. (2017). Exploiting media. Controllable chemistry leading to nanoscale metal and metal boride non-covalent π interactions for catalyst design. Nature 543, 637–646. particles. Langmuir 10, 4726–4730. doi: 10.1021/la00024a055 doi: 10.1038/nature21701
Frontiers in Chemistry | www.frontiersin.org 15 August 2020 | Volume 8 | Article 735 Couvret et al. Graphite Functionalization With Copper Phthalocyanine
Pakapongpan, S., Mensing, J. P., Phokharatkul, D., Lomas, T., and Tuantranont, Sorokin, A. B. (2013). Phthalocyanine metal complexes in catalysis. Chem. Rev. A. (2014). Highly selective electrochemical sensor for ascorbic acid based on 113, 8152–8191. doi: 10.1021/cr4000072 a novel hybrid graphene-copper phthalocyanine-polyaniline nanocomposites. Vigneron, F., Piquet, A., Baaziz, W., Ronot, P., Boos, A., Janowska, I., et al. (2014). Electrochim. Acta 133, 294–301. doi: 10.1016/j.electacta.2014.03.167 Hydrophobic gold catalysts: from synthesis on passivated silica to synthesis on Raja, R., and Ratnasamy, P. (1996). Selective oxidation with copper complexes few-layer graphene. Catal. Today 235, 90–97. doi: 10.1016/j.cattod.2014.04.016 incorporated in molecular sieves. Stud. Surf. Sci. Catal. 101, 181–190. Waikar, J., Pawar, H., and More, P. (2019). Review on CO oxidation by noble doi: 10.1016/S0167-2991(96)80228-X and non-noble metal based catalyst. Catal. Green Chem. Eng. 2, 11–24. Reis, R. M., Valim, R. B., Rocha, R. S., Lima, A. S., Castro, P. S., Bertotti, M., doi: 10.1615/CatalGreenChemEng.2019030245 et al. (2014). The use of copper and cobalt phthalocyanines as electrocatalysts Wan, H., Wang, Z., Zhu, J., Li, X., Liu, B., Gao, F., et al. (2008). Inﬂuence of CO for the oxygen reduction reaction in acid medium. Electrochim. Acta 139, 1–6. pretreatment on the activities of CuO/γ-Al2O3 catalysts in CO + O2 reaction. doi: 10.1016/j.electacta.2014.07.003 Appl. Catal. B 79, 254–261. doi: 10.1016/j.apcatb.2007.10.025 Schlierf, A., Yang, H., Gebremedhn, E., Treossi, E., Ortolani, L., Chen, L., et al. Wang, W., Zhang, Y., Sun, T., and Wang, Y.-B. (2015). On the nature of the (2013). Nanoscale insight into the exfoliation mechanism of graphene with stacking interaction between two graphene layers. Chem. Phys. Lett. 620, 46–49. organic dyes: eﬀect of charge, dipole and molecular structure. Nanoscale 5, doi: 10.1016/j.cplett.2014.12.024 4205–4216. doi: 10.1039/c3nr00258f Zhu, M., and Diao, G. (2012). High catalytic activity of CuO nanorods for Seoudi, R., El-Bahy, G. S., and El Sayed, Z. A. (2005). FTIR, TGA and DC electrical oxidation of cyclohexene to 2-cyclohexene-1-one. Catal. Sci. Technol. 2, 82–84. conductivity studies of phthalocyanine and its complexes. J. Mol. Struct. 753, doi: 10.1039/C1CY00274K 119–126. doi: 10.1016/j.molstruc.2005.06.003 Silva, H., Mateos-Pedrero, C., Ribeirinha, P., Boaventura, M., and Mendes, Conﬂict of Interest: The authors declare that the research was conducted in the A. (2015). Low-temperature methanol steam reforming kinetics over absence of any commercial or ﬁnancial relationships that could be construed as a a novel CuZrDyAl catalyst. Reac. Kinet. Mech. Cat. 115, 321–339. potential conﬂict of interest. doi: 10.1007/s11144-015-0846-z Soliman, N. K. (2019). Factors aﬀecting CO oxidation reaction over Copyright © 2020 Couvret, Genay, Robert, Michel and Caps. This is an open-access nanosized materials: a review. J. Mater. Res. Technol. 8, 2395–2407. article distributed under the terms of the Creative Commons Attribution License (CC doi: 10.1016/j.jmrt.2018.12.012 BY). The use, distribution or reproduction in other forums is permitted, provided Song, J.-J., Zhu, B.-L., Han, Q.-W., Tian, J., Zhao, W.-L., Wang, S.-R., et al. (2013). the original author(s) and the copyright owner(s) are credited and that the original NTs-supported copper oxide with improved catalytic performance for low publication in this journal is cited, in accordance with accepted academic practice. temperature CO oxidation via cerium oxide modiﬁcation. J. Chil. Chem. Soc. No use, distribution or reproduction is permitted which does not comply with these 58, 1628–1631. doi: 10.4067/S0717-97072013000100027 terms.
Frontiers in Chemistry | www.frontiersin.org 16 August 2020 | Volume 8 | Article 735